Volume 3 Paper 2
Magnetic Measurements of the Response of Corrosion Activity within Aircraft Lap Joints to Accelerated Corrosion Testing
Grant Skennerton, Afshin Abedi, Robert G. Kelly, and John P. Wikswo, Jr.
Because you are not logged-in to the journal, it is now our policy to display a 'text-only' version of the paper. This version is obtained by extracting the text from the PDF or HTML file, and it is not guaranteed that the text will be a true image of the text of the paper. The text-only version is intended to act as a reference for search engines when they index the site, and it is not designed to be read by humans!
If you wish to view the human-readable version of the paper, then please Register (if you have not already done so) and Login. Registration is completely free.
JCSE Volume 3, Paper 2
Submitted 16th March 2000, published for public review June 2000
Magnetic Measurements of the Response of Corrosion Activity within
Aircraft Lap Joints to Accelerated Corrosion Testing
Grant Skennerton (1), Afshin Abedi (1), Robert G. Kelly (2), and John P.
Wikswo, Jr. (1)
(1) Department of Physics and Astronomy, Vanderbilt University, Nashville,
TN 37235, USA
(2) Department of Materials Science and Engineering, University of Virginia
Charlottesville, VA 22903, USA
We have demonstrated the ability of Superconducting QUantum Interference
Device (SQUID) magnetometers to qualitatively monitor electrochemical activity
within lap joints removed from actual aircraft. This work lays the foundation
for quantitative measurements of corrosion rates within occluded structures.
In this study, a SQUID magnetometer was used to examine hidden corrosion
activity within lap joints removed from ageing KC-135 aircraft. During
exposure, we imaged each specimen every 60 minutes. We designed the protocol
to expose each lap joint specimen to a range of increasingly corrosive
exposure sequences. The results obtained from this protocol show that there is
a clear relationship between corrosivity of the environment and the activity
generated within the lap joint. Over a range of increasing corrosive
environments, the activity generated shows significant increases with each
step. This technique allows us to determine non-invasively the corrosivity of
the chemical environment already existing inside the lap joint relative to
environments of known corrosivity.
§2 Keywords: SQUID magnetometers, lap joints, corrosion measurement
§3 Corrosion of aircraft aluminium is a major problem for the United States
Air Force and a great deal of effort is being applied to incorporate its
effects into aircraft maintenance and structural integrity decisions. Models
used for such decisions require accurate values of the rate of corrosion
within occluded regions, such as lap joints, in a variety of operational
environments. The overall goal of this project is to ascertain the rate of
hidden corrosion in lap joints specimens removed from ageing aircraft under
controlled environmental conditions.
§4 A limitation common to the existing corrosion measurement techniques is
their inability to probe accurately the instantaneous rate of corrosion within
lap joints or beneath thick layers of paint or specialised military coatings.
This barrier has prevented incorporation of corrosion into the Aircraft
Structural Integrity Program (ASIP). As a result, studies of these phenomena
typically require the creation of redundant samples that are examined
destructively at regular intervals throughout the duration of test. Until now,
instantaneous rates of hidden corrosion, their spatial distribution within a
structure and how the environment affects those rates could not be determined
by existing techniques.
§5 Unlike the variety of techniques presently utilised, such as atmospheric
exposure, electrochemical techniques and NDE techniques, SQUIDs possess the
ability to measure rate instantaneously, and do not need to integrate
corrosion damage over long periods of time to determine corrosion rates.
Preliminary work at Vanderbilt [1-4] using SQUIDs to monitor currents from
either exposed or hidden corrosion demonstrated the SQUIDs' utility for the
periodic, non-destructive analysis of corrosion test specimens for which the
corrosion activity is not directly accessible. Their unparalleled sensitivity,
spatial resolution (microns to millimetres), and DC-to-10 kHz bandwidth allows
SQUIDs to map steady or time-varying currents deep within a sample without
having to make contact with the sample. In addition, SQUIDs do not require
visualisation of or other direct access to the metal surface that is
2.1 SQUID System
§6 We have developed instrumentation, recording, and analysis techniques that
are optimised for the measurement of the spatial and temporal dependence of
the magnetic fields associated with hidden corrosion in lap joints. Our two
corrosion mapping systems [5,6] use SQUID gradiometers and each include a
magnetic shield, a scanning stage with a custom sample-handling system, a
computer control system, and custom scanning and analysis software.
2.2 Specimen Design
§7 Four aluminium lap joint specimens were obtained from retired KC-135
aircraft. The specimens were approximately 250 mm long, had three fastener
(rivet) rows, and were three fasteners wide (plus half the fastener pitch on
each side). The majority of the free-standing stringer material was cut off.
The total height of each specimen at the stringer was approximately 10 mm. All
exposed metal surfaces were painted with MIL-P-23377 epoxy primer and
MIL-PRF-85285 polyurethane top coat. The paint was applied with a paint spray
gun in the same manner the aircraft are painted. The edges were sealed with
low-adhesion polysulfide sealant so hydration could only occur from the two
mouths of the lap joint. Holes were drilled and countersunk in the ends of the
lap joint for accommodating 4-40 flat-head nylon screws as shown in Figure 1.
These holes were used to fasten the lap joints to the specimen chamber.
§8 Figure 1: Schematic diagram of a typical lap joint specimen.
2.3 Corrosion Chambers
§9 We designed environmental chambers that allowed us to expose lap joints to
a variety of environments while we scanned them under the SQUID. After
attachment of the samples and baseline SQUID scanning, we introduced the
various gaseous or liquid environments to the chamber. We did not remove the
lap joints from the chamber or from the magnetic shield until the test was
2.4 Accelerated Corrosion Methodology
§10 To determine the chloride-dependence of corrosion within the lap joint, and
to examine experiment repeatability and cycling effects, we designed a
protocol that exposed each lap joint specimen to a range of increasingly
corrosive exposure sequences. These sequences are shown in Table 1. Each
sequence, or "step," was six days in duration. We applied three
passes of each step to each specimen before progressing to the next step in
the protocol. At the beginning of each pass, we baked the specimen at 50�C in
a vacuum oven for three days to dehydrate the sample and halt any ongoing
corrosion. Prior to scanning, we degaussed the specimen in order to provide a
background level that was repeatable over multiple passes. To quantify the
background magnetic field of the lap joints, we scanned samples in dry
nitrogen gas for 24 hours. We then exposed the specimen to a corrosive
environment for 48 hours. We intended that the corrodent used in each
subsequent step was more corrosive than the one used in the previous step.
During step 1, we exposed specimens to humid air. During step 2, distilled
water was used to provide a measure of the corrosivity of the material already
present in the lap joint. Steps 3 and 4 used 0.01 M Cl- and 0.1 M
Cl- respectively. We only completed one pass of step 4.
Table 1: Exposure sequence of lap joint
protocol III. We repeated each step twice.
Vacuum bake (3 days), degauss, dry
(1 day), 98% RH (2 days)
Vacuum bake (3 days), degauss, dry N2 (1
day), distilled water (2 days)
Vacuum bake (3 days), degauss, dry N2 (1
day), 0.01M NaCl (2 days)
Vacuum bake (3 days), degauss, dry N2 (1
day), 0.1M NaCl (2 days)
2.5 Magnetic Field Metrics
§11 We define several useful magnetic field metrics in a previous paper .
Briefly, the background magnetic field image, BG, is defined as the
spatial average of K dry scan images (raster scans) at a fixed height
above the dry (non-corroding) sample.
Here Bz represents the average magnetic flux density
measured over the area of the z-axis pickup-coil of the magnetometer, xi
and yj represent the position of the (i,j)th
pixel with respect to the scanning co-ordinates, K represents the
number of dry scans to be averaged, tk denotes the starting
time of the kth scan and is measured with respect to the
beginning of the first scan of the experiment, and Dt
represents the time it takes to finish a single raster scan and is a constant
for all the scans taken in one experiment. The notation in this and the
following equations contains Dt in
order to remind the reader that we acquired each raster image in a time
interval [tk , t+Dt].
§12 After recording a stable background, we introduced the corrosive solution
to the sample. The resulting change in magnetic field with respect to BG
we refer to as Bcorr and define (2).
where k represents the kth magnetic field
image. The Magnetic Activity (MA) of the sample, recorded in the kth
scan of the experiment, is defined as the absolute value of (2), and
represents the absolute change in magnetic field due to corrosion with respect
to the non-corroding (dry) background image.
§13 Furthermore, we define the Spatially Integrated Magnetic Activity (SIMA)
where we take the summations over all the pixels in the kth
image, and Dx and Dy
represent the distance between two consecutive pixels in the corresponding
scan direction. SIMA(tk,Dt)
is a number proportional to the net magnetic activity of the sample as
recorded during the kth scan, and should be proportional to
the net corrosion activity of the sample during this time-interval (i.e.,
[tk , tk+Dt]).
The graph of SIMA(t,Dt) versus
time represents the time-course of corrosion activity of the sample.
§14 Since SIMA(tk,Dt)
is proportional to the net corrosion current (and hence the mass-loss rate) in
the kth image, then the area under the curve SIMA(t,Dt)
versus time must be proportional to the total mass-loss of the sample during
the corrosion experiment. For an experiment consisting of K
raster scans, we define this quantity as the Temporally Summed SIMA
§15 In the case where SIMA is proportional to mass-loss rate, TSSIMA
should be proportional to the total mass-loss of the sample during the
§16 Finally, to determine the cumulative magnetic activity at each pixel for
the course of the experiment, we define the Temporally Summed Magnetic
Activity (TSMA) at point (xi,yj) as
where T is the length of time that the sample was exposed to
corrosive solution. Therefore, TSMA(x,y) is a two-dimensional image,
wherein each pixel is the time-weighted cumulative measure of the magnetic
activity of that pixel throughout the experiment, and hence will spatially
identify the regions with differing net magnetic activity.
2.6 Removal of Magnetic Contamination
§17 Before we computed final quantitative metrics, we processed the data to
minimise the influence of magnetic contamination on the calculated corrosion
activity. We observed localised regions of high magnetic activity within the
scan's area, and the time-course of magnetic activity in these regions was
often different from the time-course of activity in the rest of the corroding
sample. The spatio-temporal property of this activity is consistent with
behaviour we have observed for the corrosion of localised ferro-magnetic
contaminants. As these localised regions were not necessarily within the area
of the specimen, it cannot be assumed that these signals are associated with
localised distribution of corrosion current sources. Because of this, we
removed the magnetic contribution of these localised particles from that of
the corroding samples in order to have proper measurements of the
corrosion-related changes in magnetic activity.
§18 We used a post-processing technique based on temporal-correlation to
distinguish and then remove the contaminated regions from the data. Once we
identified a pixel as exhibiting time-dependent magnetic contamination, we
correlated the time-course of that pixel's magnetic activity with the
time-course of all other pixels in the image. The correlation coefficient, S,
of the contaminant pixel (A) with another pixel (B) is:
§19 All pixels whose cross-correlation with contamination exceeded a
predetermined threshold were eliminated from the calculation of quantitative
metrics. Using this user-controlled threshold limit, we generated a mask and
applied this to the data. We zeroed the magnitude of the magnetic activity of
pixels with correlation coefficients greater than or equal to the threshold
limit. We did not change the magnitude of activity of pixels with correlation
coefficients less than the threshold limit. Though some loss of data is
unavoidable, the post-processing technique has proved to be a viable technique
for studying magnetically contaminated samples. In the future, we expect to
improve the method used for identifying and eliminating contaminated areas
from the data.
§20 This procedure is demonstrated in Figure 2. Figure 2(a) is a TSMA
image obtained from lap joint SM11-SP1. We identify region A as one typical of
contamination, while we identify region B as one typical of the lap joint's
true activity. Figure 2(b) shows the magnitude of the dipolar contamination
source along section X-X. The dipole is clearly much greater in magnitude than
other areas along section X-X. Figure 2(c) shows the time-course of the
magnetic activity of region A. Figure 2(d) shows the time-course of the
magnetic activity of region B. Comparison of Figure 2(c) and 2(d) shows the
marked difference between the contaminated and uncontaminated reigions, both
in magnitude and nature of the magnetic activity. Figure 2(e) shows the mask
generated by an 80% cross-correlation of the data with region A. Once the mask
is applied, Figure 2(f) shows the magnitude of the dipolar contamination
source along section X-X after masking. Comparison of Figure 2(b) with 2(f)
demonstrates the success of this masking technique in removing the signal of a
contaminant source from the data.
§21 Figure 2: (a) The TSMA image from lap-joint SM11-SP1. We
identified region A as contamination. We identified region B as a region
typical of the lap joint's activity. (b) The magnitude of the dipolar
contamination source along section X-X. (c) The time-course of magnetic
activity in region A. (d) The time-course of activity in region B. (e) The
mask generated by an 80% correlation of the data with region A. (f) The effect
of masking on the region A along section X-X.
2.7 Statistical Analyses
§22 Our statistical analysis of the data involved a test of the significance on
the mean . In all cases, we hypothesised that environmental changes under
either protocol would produce no significant change in magnetic activity, i.e.,
the ratio of the activity before the transition to the activity after the
transition would be unity, or 1 (m0
= 1). Thus our null hypothesis can be written: H0: m
= m0, i.e., the population
mean (m) was expected to be equal to m0.
Each protocol was analysed independently. The selected significance level was
1%, or a = 0.01. In testing the significance of the
mean, we reject the null hypothesis if the probability (P) of the observed
difference between m and m0
is less than a (0.01), which is to say that m
is not compatible with m0. In
such a case, variation in the sample population is not able to explain the
difference between the null hypothesis value and the sample values. However,
should P exceed the significance level of 0.01, we expected that there is no
significant difference between m and m0.
3 Results and Discussion
3.1 Dynamics of Magnetic Activity
§23 We examined four KC-135 lap joints in Protocol III (Sample 11 Specimens 1
through 4). SIMA versus time curves obtained from each are shown in
Figures 3 to 6 respectively. In each step, upon introduction of the corrodent
at 24 hours, the magnetic activity increased. For step 1 (exposure to 98% RH
air), the new level reached is constant over the 48 hour period when compared
to the levels reached in steps 2 to 4 (exposure to solutions). We observed
transients in the level of activity that did not coincide with changes in the
corrosive. We observed this behaviour in specimens exposed under earlier
comment(24)Figure 3: SIMA versus time curves obtained from KC-135 SM11-SP1.
Figure 4: SIMA versus time curves obtained from KC-135 SM11-SP2.
comment(25)Figure 5: SIMA versus time curves obtained from KC-135 SM11-SP3.
comment(26)Figure 6: SIMA versus time curves obtained from KC-135 SM11-SP4.
§27 For each lap joint, we calculated the average SIMA for the 24-hour period
that we held the specimen in dry N2. We also calculated the average
SIMA for the 48-hour period that we exposed the specimen to corrodent. Figure
7 shows the ratio of the average SIMA of the corrosive environment to the
average SIMA obtained during exposure to dry nitrogen averaged over all lap
joints for each step. We hypothesised that the corrodent would have no
significant effect on the magnetic activity within the lap joint, i.e.,
that there would be no increase (H0: ratio = 1). We tested
our null hypothesis using the populations of SIMA ratios obtained in each
step. Table 2 shows that introduction of corrodent produces a statistically
significant increase in activity in the lap joints (P<0.01). As shown the
level of activity achieved during corrosion in each step increases relative to
the earlier steps. During step 2, the level of SIMA attained during exposure
to the corrodent was 2.6 times greater than that attained in step 1, step 3
2.1 times greater than step 2, and step 4 1.4 times greater than step 3.
§28 Figure 7: Average increases in activity upon humidification/immersion of
KC-135 SM11 lap joint specimens. The figure shows the inter-step increase in
Table 2: Average increases in activity upon
humidification or immersion of KC-135 SM11 lap joint specimens, and the
statistical significance calculated for this increase. H0:
ratio = 1, a =
3.2 Cumulative Magnetic Activity Generated in Protocol III
§29 Table 3 shows the average TSSIMA obtained during each step for each
lap joint. Figure 8 shows an upward trend in activity over the four passes.
These data are consistent with the relationship seen in the SIMA data,
discussed above. Figure 9 shows the average TSSIMA obtained from each
step. This figure shows a clear upward trend in TSSIMA as the
environment becomes more corrosive. However, the increase in activity between
steps 3 and 4 is not as pronounced. We tested the significance the increase in
TSSIMA seen between steps. We hypothesised that there would be no
significant increase in TSSIMA, i.e., the ratio would be unity (H0:
ratio = 1, a = 1%). Table 4 presents the ratios of TSSIMA
from step to step and the significance of this increase. As can be seen, the
increase in activity from step 1 (98% RH) to step 2 (distilled water) is
significant, as is the increase from step 2 to step 3 (0.01 M Cl-).
The significance levels for these ratios are <0.0001 and 0.0044
respectively, which are both below our significance level of 0.01. The ratio
of TSSIMA between step 4 and step 3 is only 1.1, or an increase of 10%.
As expected, this increase was calculated to not be significant (P =
0.32). However, as we took only four data points in step 4, we cannot assume
this last observation to be definitive.
Table 3: TSSIMA data from KC-135 lap
joint specimens averaged over each step. The table also shows the average TSSIMA
for all four lap joints for each step. (TSSIMA � sTSSIMA
8 � 4
23 � 13
37 � 5
11 � 2
28 � 10
39 � 4
9 � 2
34 � 15
52 � 19
6 � 1
29 � 14
42 � 3
8 � 3
28 � 14
43 � 12
46 � 12
§30 Figure 8: TSSIMA data of KC-135 lap joint specimens averaged over three
§31 Figure 9: Average TSSIMA data of each step of Protocol III. Average
inter-step increases in TSSIMA of KC-135 SM11 lap joint specimens, and
their probability (H0:
ratio = 1, a = 1).
§32 We designed a protocol to determine the effects of moisture and chloride on
lap joints relative to the initial condition of a dry, inactive joint. We
exposed lap joint specimens to what we anticipated was a range of increasingly
corrosive exposure sequences: humid air, distilled water, 0.01 M Cl-,
and 0.1 M Cl-. In between each exposure, we effectively
"reset" the specimens by baking them in a vacuum and degaussing
before the subsequent exposure. We show that the SQUID has sufficient
sensitivity to detect corrosion activity within the joint upon exposure to
only humid air. By then immersing the lap joints in distilled water, we have
observed the corrosivity of the chemical environment existing inside the lap
joint. We show that distilled water generates significantly more activity than
§33 Upon exposure to 0.1 M Cl-, we show chloride to generate
significantly more activity than the natural conditions with the lap joint, as
brought out by the distilled water. However, there was no statistically
significant difference between the activity generated in 0.01 M Cl-
and that generated in 0.1 M Cl-. Hence we conclude that SQUIDs are
capable of making quantitative measurements of the relative rates of corrosion
of aircraft lap joints under differing conditions of humidity and chloride.
§34 We have yet to obtain the calibration of mass-loss to magnetic-signal for
lap joint specimens. Although we have established a quantitative calibration
between magnetic signal and corrosion rate for other geometries, its use for
lap joints is currently under study. Hence, we present a magnetic measurement
that can be used to compose the corrosion rate under different circumstances,
but it is not yet possible to use these data for quantitative assessment of
absolute corrosion rates. In the future we will be conducting experiments to
determine the mass-loss to magnetic field calibration for specimens of lap
§35 Although magnetic contamination had been previously thought to be a
limiting factor in the use of SQUIDs to study corrosion activity in aircraft
samples, we show that the problems of magnetic contamination can in general be
overcome by selection of samples without ferromagnetic fasteners, modest care
in sample preparation, thorough degaussing of the samples at the beginning of
each step in the exposure protocol, subtraction of time-independent background
fields, and masking of the regions of the magnetic images that show a time
course consistent with the corrosive activity of ferromagnetic contaminants.
While work will continue to refine this technique, we demonstrate clearly that
high-quality corrosion data can be obtained from samples removed from aging
§36 This work was funded in part through Air Force contract F09603-97-C-0050,
"Corrosion/Fatigue Effects on Structural Integrity," issued through
the Air Force Corrosion Office (AFCO) at Robins Air Force Base in Warner
Robins, GA, NCI Information Systems, Inc., and Air Force Research Laboratory
(AFRL). We thank Garth Cooke and Jim Suzel (NCI), Deborah Peeler (AFRL), and
Richard Kinzie (AFCO) for their comments and suggestions regarding the
experimental design and these measurements. We thank Steve Kaldon (NCI) for
provision of the lap joint samples.
J.P. Wikswo, Jr., "SQUID Magnetometers for Studying Corrosion and
Corrosion Protection in Aircraft Aluminium", NACE International,
Paper No. 293, pp. 1-17 (1997).
D. Li, Y.P. Ma, W.F. Flanagan, B.D. Lichter, & J.P. Wikswo, Jr.,
"Application of Superconducting Magnetometry in the Study of Aircraft
Aluminium Alloy Corrosion", Corrosion, 52 (3): 219-231 (1996).
D. Li, Y.P. Ma, W.F. Flanagan, B.D. Lichter, & J.P. Wikswo, Jr.,
"Detecting In-Situ Active Corrosion by a SQUID Magnetometer",
Journal of Minerals, Metals and Materials, 47 (9): 36-39 (1995).
D. Li, Y.P. Ma, W.F. Flanagan, B.D. Lichter, and J.P. Wikswo, Jr.,
"The Use of Superconducting Magnetometry to Detect Corrosion in
Aircraft Alloys", Proceedings of the Tri-Service Conference on
Corrosion, Orlando, FL, pp. 335-346 (June 1994).
A. Abedi, J. Fellenstein, A. Lucas, & J. Wikswo Jr., "A SQUID
Magnetometer System for Quantitative Analysis and Imaging of Hidden
Corrosion Activity in Aircraft Aluminium Structures", Rev. Sci.
Instrum., in press.
D.S. Buchanan, D.B. Crum, D. Cox, T.H. Aukerman, T.A. Sager, & J.P.
Wikswo Jr., in Advances in Biomagnetism, eds. S.J. Williamson, G. Hoke, G.
Stroink, & M. Kotani (NY: Plenum Press, 1990), pp. 667-679.
A. Abedi, J. P. Wikswo Jr., "Magnetic Field as a Quantitative
Measure of Ongoing Corrosion", submitted for publication, (1999).
T. Colton, "Statistics in Medicine", Little, Brown &
Company, Boston, MA, p. 116 (1974).